# Tof-SIMS spectra of historical inorganic pigments: Copper-, zinc-, arsenic-, and phosphorus-containing pigments in positive polarity

Caroline Bouvier, Sebastiaan van Nuffel, Alain Brunelle

► To cite this version:

Caroline Bouvier, Sebastiaan van Nuffel, Alain Brunelle. Tof-SIMS spectra of historical inorganic pigments: Copper-, zinc-, arsenic-, and phosphorus-containing pigments in positive polarity. Surface Science Spectra, 2024, 31 (2), pp.025001. 10.1116/6.0003722. hal-04637506

HAL Id: hal-04637506

https://hal.science/hal-04637506v1

Submitted on 6 Jul 2024

HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-
entific research documents, whether they are pub-
lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

L'archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d'enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

<figure><img src="image_1.png" /></figure>

Distributed under a Creative Commons Attribution 4.0 International License
# Tof-SIMS spectra of historical inorganic pigments: Copper-, zinc-, arsenic-, and phosphorus-containing pigments in positive polarity 🤔

Special Collection: ToF-SIMS Spectra of Historical Inorganic Pigments

Caroline Bouvier 🐦 ; Sebastiaan Van Nuffel 🐦 ; Alain Brunelle 📄

<figure><img src="image_2.png" /></figure>

Check for updates

Surf. Sci. Spectra 31, 025001 (2024)

https://doi.org/10.1116/6.0003722

<figure><img src="image_3.png" /></figure>

View
Online

<figure><img src="image_4.png" /></figure>

Export
Citation
# Tof-SIMS spectra of historical inorganic pigments: Copper-, zinc-, arsenic-, and phosphorus-containing pigments in positive polarity

<figure><img src="image_5.png" /></figure>

Cite as: Surf. Sci. Spectra 31, 025001 (2024); doi: 10.1116/6.0003722

Submitted: 27 April 2024 · Accepted: 18 June 2024 ·

Published Online: 3 July 2024

<figure><img src="image_6.png" /></figure>

View Online

<figure><img src="image_7.png" /></figure>

Export Citation

<figure><img src="image_8.png" /></figure>

CrossMark

Caroline Bouvier,<fnref n="1" />,<fnref n="2" /> ID Sebastiaan Van Nuffel,<fnref n="2" />,<fnref n="3" /> ID and Alain Brunelle<fnref n="1" />,ª ID

## AFFILIATIONS

**Note:** This paper is part of the 2024 Special Topic Collection on ToF-SIMS Spectra of Historical Inorganic Pigments.

ªAuthor to whom correspondence should be addressed: alain.brunelle@cnrs.fr

## ABSTRACT

Time-of-flight secondary ion mass spectrometry (ToF-SIMS) is increasingly used to analyze cultural heritage materials because it can simultaneously detect organic and inorganic materials while mapping them on a surface. The precise identification of a pigment in a specific layer of a painting or of remaining color on a statue can inform about the technique used or the time of manufacture as well as expose possible forgeries when anachronistic ingredients are identified. Reference spectra are required to confidently identify a given pigment using ToF-SIMS. This paper focuses on eight pigments containing copper, zinc, arsenic, or phosphate, all manufactured following historical recipes. The positive polarity ToF-SIMS reference spectra using a $Bi_3^+$ primary ion species are presented here. Presented together, these spectra and corresponding tables of secondary ions provide a valuable help in differentiating these pigments, because copper, zinc, arsenic, or phosphate, combined with oxygen, share many mass interferences.

© 2024 Author(s). All article content, except where otherwise noted, is licensed under a Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/). https://doi.org/10.1116/6.0003722

Accession#: 01939, 01940, 01941, 01942, 01943, 01944, 01945, 01946

Technique: SIMS

Specimen: Peach black, Bone black, Realgar, Bristol yellow medium, Azurite, Malachite, Verdigris, Zinc white

Instrument: IONTOF, TOF SIMS IV

Major Species in Spectra: O, H, C, Cu, Zn, P, Ca, As, S, V, Bi, Cl

Minor Species in Spectra: Hydrocarbon contamination

Published Spectra: 8

Spectral Category: Reference

## INTRODUCTION

ToF-SIMS imaging can detect a wide range of elements, so colored minerals can be identified and mapped, given that reference spectra are available for reliable assignment. This paper provides a comparative ToF-SIMS spectral database for eight historical inorganic pigments, containing copper carbonate, zinc oxide or phosphates, vanadium oxide, calcium phosphates, or arsenic sulfide. Numerous possibilities for mass interferences exist between combinations of these elements. Without being able to refer to comparative datasets that provide an overview of the fragment ions for each pigment, it would be difficult to accurately identify one of them as an unknown pigment.

The reference materials were supplied by specialized manufacturers selling pigments reproducing historical recipes as closely as possible, such as Kremer Pigmente GmbH. Pigments were available as finely ground powder of variable particle size (between one and a few tens of µm) conditioned in glass sealed vials. In paintings, pigment particles are dispersed in the binder and not dissolved, so all references were analyzed without any preparation treatment. Natural and synthetic pigments may contain impurities, and specimen compositions described below are the major components as found on the material data sheets provided by the suppliers.

<footnote n="1">¹Sorbonne Université, CNRS, Laboratoire d'Archéologie Moléculaire et Structurale (LAMS), Paris 75005, France</footnote>

<footnote n="2">²Maastricht MultiModal Molecular Imaging Institute (M4i), Maastricht University, Maastricht 6229ER, The Netherlands</footnote>

<footnote n="3">³Faculty of Science and Engineering, Maastricht University, Maastricht 6229EN, The Netherlands</footnote>
A stainless-steel spatula was cleaned with propan-2-ol and the powder was directly deposited on a 1 × 1 mm² piece of conductive double-sided tape (3M Electrically Conductive Adhesive Transfer Tape 9703) already fixed to a 1 cm × 1 cm × 0.125 mm stainless steel plate (17-7PH, Goodfellow Cambridge Limited, UK) fitting the dimensions of the sample holder. A hand press covered with clean aluminum foil was applied onto the powder to fix it to the tape. This allowed to operate in the analysis chamber under ultra-high vacuum (10⁻⁸–10⁻⁹ hPa) while ensuring a flat surface. For highly toxic pigments, such as the arsenic sulfide Realgar (#01941), a pellet with a flat surface was prepared using a press (Mini-Pellet Press P/N GS03940, Specac Ltd, UK) to limit dust formation.

All spectra were obtained on an IONTOF TOF SIMS IV equipped with a 25 keV bismuth liquid metal ion gun and an Argon gas cluster ion beam (GCIB). Before all analyses, a 500 × 500 µm² surface was cleaned using 1500–2000 Ar clusters with a kinetic energy of 20 keV (sputter ion dose 2 × 10¹⁵ ions/cm²). Analyses were then performed on a 250 × 250 µm² area centered in this larger cleaned area, rastered over 128 × 128 pixels using the high current bunched mode. The primary ion dose (25 keV Bi³⁺) was 4.35 × 10¹¹ ions/cm². Surface potential was compensated and charging of the sample was compensated with the low-energetic 20 eV electrons of the flood gun.

Data were calibrated using sets of peaks as similar as possible for all spectra, using peaks that could be confidently identified. Potassium, copper, zinc, and calcium have distinctive isotopic patterns ensuring confident attribution of the peaks, so #01939 data were calibrated using lists including potassium-containing ions K⁺, K₂⁺, K₂OH⁺, and K₂Cl⁺; #01943, #01944, and #01945 data were calibrated using lists including Na⁺, Cu⁺, Cu₂OH⁺, and Cu₃O⁺ ions; and #01946 data were calibrated using Na⁺, Zn⁺, Zn₂O₃⁻, Zn₃O₃⁻, ⁶⁶Zn⁶⁸ZnZn₂O₄⁺, and ⁶⁶Zn⁶⁸ZnZn₃O₅⁺. Both #01940 and #01942 were calibrated using calcium-containing ions including Ca⁺ and Ca₂O⁺. No bismuth and vanadium-containing ions were used to calibrate #01942 data, since bismuth has no isotope and is close in mass to VP₂O₆. Arsenic sulfide #01941 data were calibrated using ions having high intensity, namely, As⁺, AsS⁺, As₂S₂⁻, AsPbS⁺, and As₃S₃⁻ ions. These calibration lists allowed for a good coverage of the mass range of interest for each specimen, and they are fully detailed in the corresponding tables below.

Pigments contain diverse metallic oxides, hydroxides, carbonates, and even hydrocarbons. They are found inside painting layers that are mostly organic materials. All these compounds do not follow the same ionization processes and have different ionization kinetics.¹ In this context, the choice for the calibration ions is a crucial step to ensure proper peak attribution. If the analytical question aims at identifying the nature of a pigment particle, then the calibration must include inorganic ions, such as the list above, spanning all the mass range of interest, and if possible of the same ion family as those of interest. However, if the analytical question focuses mainly on the identification of organic materials, the calibration must include known low-mass hydrocarbon ions (such as C₂H₃⁺, C₃H₅⁺, C₄H₇⁺, and C₇H₇⁻). The safest strategy when interpreting data from a painting cross-section would be to rely on several calibration sets adapted to the ions of interest and that can be confidently defined independently of the sample's unknowns.

Figures and tables presented below contain the major peaks for positive polarity. Each pigment is uniquely identified thanks to an accession number and they are grouped according to their composition and described in the following section. Their historical relevance is briefly described based on the current literature.²⁻⁶ Spectrum ID# refers to that number.

## SPECIMEN DESCRIPTION (ACCESSION # 01939)

**Specimen:** Peach black (Kremer Pigmente Ref. 12010)

**CAS Registry #:** Unknown

**Specimen Characteristics:** Unknown homogeneity; solid; amorphous; dielectric; inorganic compound; powder;

**Chemical Name:** Amorphous carbon

**Source:** Kremer Pigmente GmbH

**Specimen Composition:** Amorphous carbon (charred peach kernel)

**Form:** Ground pigment powder

**History and Significance:** Black pigments derived from charcoals are rarely detectable by the analytical techniques used to investigate pigments such as XRF, while carbon-based black pigments have been used in every society since the domestication of fire. Peach black, for instance, only requires the calcination of kernels. Identifying this pigment is of interest, as they are omnipresent in historical artistic practice. ToF-SIMS is able to map and identify micrometric particles of carbon-based pigments.

**As Received Condition:** Ground pigment powders were stored in a sealed glass vial in a wooden box, protected from daylight. Stored at room temperature.

**Analyzed Region:** Areas of 250 × 250 µm²

**Ex Situ Preparation/Mounting:** Powder was deposited and pressed onto conductive double-sided tape attached to stainless steel 1 × 1 cm² plates. The resulting deposit of powder had a flat surface and was fixed in a suitable way for the vacuum chamber. The plate was directly mounted on a “backmount” sample holder (IONTOF).

**In Situ Preparation:** None

**Charge Control Conditions and Procedures:** A low energy electron flood gun was used. Bias voltage between 20 and −30 V. Flood gun filament current 2.35 A. Surface potential was corrected (sample dependent).

**Temp. During Analysis:** 300 K

**Pressure During Analysis:** Between 1 × 10⁻⁵ and 1 × 10⁻⁶ Pa

**Pre-analysis Beam Exposure:** Ar₁₅₀₀–₂₀₀₀, 20 keV, 2 × 10¹⁵ ions/cm²

## SPECIMEN DESCRIPTION (ACCESSION # 01940)

**Specimen:** Bone black (Kremer Pigmente Ref. 47100)

**CAS Registry #:** 8021-99-6

**Specimen Characteristics:** Unknown homogeneity; solid; amorphous; dielectric; inorganic compound; powder;

**Chemical Name:** Bone charcoal

**Source:** Kremer Pigmente GmbH

**Specimen Composition:** Amorphous carbon, calcium phosphates

**Form:** Ground pigment powder

**History and Significance:** Bone black is made by carbonization of animal bones at temperatures over 400 °C but not above 800 °C. It mainly consists of calcium phosphate and carbonized
organics. It is very frequently used in paintings, especially in preparation layers.

**As Received Condition:** Ground pigment powders were stored in a sealed glass vial in a wooden box, protected from daylight. Stored at room temperature.

**Analyzed Region:** Areas of $250 \times 250 \mu m^2$

**Ex Situ Preparation/Mounting:** Powder was deposited and pressed onto conductive double-sided tape attached to stainless steel $1 \times 1 cm^2$ plates. The resulting deposit of powder had a flat surface and was fixed in a suitable way for the vacuum chamber. The plate was directly mounted on a “backmount” sample holder (IONTOF).

**In Situ Preparation:** None

**Charge Control Conditions and Procedures:** A low energy electron flood gun was used. Bias voltage between 20 and -30 V. Flood gun filament current 2.35 A. Surface potential was corrected (sample dependent).

**Temp. During Analysis:** 300 K

**Pressure During Analysis:** Between $1 \times 10^{-5}$ and $1 \times 10^{-6}$ Pa

**Pre-analysis Beam Exposure:** $Ar_{1500-2000}$, 20 keV, $2 \times 10^{15}$ ions/cm$^2$

## SPECIMEN DESCRIPTION (ACCESSION # 01941)

**Specimen:** Realgar/red orpiment (Kremer Pigmente Ref. 10800)

**CAS Registry #:** 1303-33-9

**Specimen Characteristics:** Unknown homogeneity; solid; unknown crystallinity; dielectric; inorganic compound; powder;

**Chemical Name:** Arsenic (III) sulfide (natural mineral)

**Source:** Kremer Pigmente GmbH

**Specimen Composition:** Natural arsenic sulfide $\alpha$-As$_4$S$_4$

**Form:** Ground pigment powder

**History and Significance:** A mineral prized for its bright red color that was used until the beginning of the 19th century. Found in volcanic and geothermal regions, and its geographic origin varies. It was found in luxurious articles in antiquity to show opulence and was used as ritual offerings and in cosmetics, despite its high toxicity. It exists in rare natural and synthetic forms. Its occurrence is difficult to investigate due to light instability, converting it to yellow pararealgar ($As_4S_4$), thereby often mistaken for other yellow As pigments unless crystalline phases can be differentiated by the analytical techniques used. Red realgar can be found in environments where the absence of light preserves it.

**As Received Condition:** Ground pigment powders were stored in a sealed glass vial in a wooden box, protected from daylight. Stored at room temperature.

**Analyzed Region:** Areas of $250 \times 250 \mu m^2$

**Ex Situ Preparation/Mounting:** Because of the toxicity of arsenic sulfide, a pellet was prepared using a Specac Mini Pellet Press. A flat surface was obtained, and dust formation was limited when handling the sample. The pellet was directly mounted on a “backmount” sample holder (IONTOF).

**In Situ Preparation:** None

**Charge Control Conditions and Procedures:** A low energy electron flood gun was used. Bias voltage between 20 and -30 V. Flood gun filament current 2.35 A. Surface potential was corrected (sample dependent).

**Temp. During Analysis:** 300 K

**Pressure During Analysis:** Between $1 \times 10^{-5}$ and $1 \times 10^{-6}$ Pa

**Pre-analysis Beam Exposure:** $Ar_{1500-2000}$, 20 keV, $2 \times 10^{15}$ ions/cm$^2$

## SPECIMEN DESCRIPTION (ACCESSION # 01942)

**Specimen:** Bristol yellow medium (Kremer Pigmente Ref. 43111)

**CAS Registry #:** 7779-90-0, 14059-33-7

**Specimen Characteristics:** Inhomogeneous; solid; unknown crystallinity; dielectric; inorganic compound; powder;

**Chemical Name:** Trizinc bis(ortho)phosphate + Bismuth vanadium tetraoxide

**Source:** Kremer Pigmente GmbH

**Specimen Composition:** $Zn_3(PO_4)_2 + BiVO_4$

**Form:** Ground pigment powder

**History and Significance:** Due to their toxicity, lead pigments have been gradually prohibited over the past two centuries. Alternative yellow pigments such as modified bismuth yellows (Bristol yellows) were produced to replace them. Bristol yellows have been used since the 20th century to imitate Naples yellow as they have similar optical properties. Copper and zinc compounds can have mass interference with Bristol Yellow ions, so their distinction is of interest.

**As Received Condition:** Ground pigment powders were stored in a sealed glass vial in a wooden box, protected from daylight. Stored at room temperature.

**Analyzed Region:** Areas of $250 \times 250 \mu m^2$

**Ex Situ Preparation/Mounting:** Powder was deposited and pressed onto conductive double-sided tape attached to stainless steel $1 \times 1 cm^2$ plates. The resulting deposit of powder had a flat surface and was fixed in a suitable way for the vacuum chamber. The plate was directly mounted on a “backmount” sample holder (IONTOF).

**In Situ Preparation:** None

**Charge Control Conditions and Procedures:** A low energy electron flood gun was used. Bias voltage between 20 and -30 V. Flood gun filament current 2.35 A. Surface potential was corrected (sample dependent).

**Temp. During Analysis:** 300 K

**Pressure During Analysis:** Between $1 \times 10^{-5}$ and $1 \times 10^{-6}$ Pa

**Pre-analysis Beam Exposure:** $Ar_{1500-2000}$, 20 keV, $2 \times 10^{15}$ ions/cm$^2$

## SPECIMEN DESCRIPTION (ACCESSION # 01943)

**Specimen:** Azurite (Kremer Pigmente Ref. 10207)

**CAS Registry #:** 12069-69-1

**Specimen Characteristics:** Inhomogeneous; solid; unknown crystallinity; dielectric; inorganic compound; powder;

**Chemical Name:** Basic copper (II) carbonate

**Source:** Kremer Pigmente GmbH

**Specimen Composition:** $Cu_3(CO_3)_2(OH)_2$

**Form:** Ground pigment powder

**History and Significance:** A natural blue to turquoise-blue-green copper carbonate that results from the erosion of copper deposits. It was used in many contexts over the centuries and was considered a fairly precious material.
**As Received Condition:** Ground pigment powders were stored in a sealed glass vial in a wooden box, protected from daylight. Stored at room temperature.

**Analyzed Region:** Areas of $250 \times 250 \ \mu m^2$

**Ex Situ Preparation/Mounting:** Powder was deposited and pressed onto conductive double-sided tape attached to stainless steel $1 \times 1 \ cm^2$ plates. The resulting deposit of powder had a flat surface and was fixed in a suitable way for the vacuum chamber. The plate was directly mounted on a “backmount” sample holder (IONTOF).

**In Situ Preparation:** None

**Charge Control Conditions and Procedures:** A low energy electron flood gun was used. Bias voltage between 20 and -30 V. Flood gun filament current 2.35 A. Surface potential was corrected (sample dependent).

**Temp. During Analysis:** 300 K

**Pressure During Analysis:** Between $1 \times 10^{-5}$ and $1 \times 10^{-6}$ Pa

**Pre-analysis Beam Exposure:** $Ar_{1500-2000}$, 20 keV, $2 \times 10^{15}$ ions/cm$^2$

## SPECIMEN DESCRIPTION (ACCESSION # 01944)

**Specimen:** Malachite, natural (Kremer Pigmente Ref. 10300)

**CAS Registry #:** 1319-53-5

**Specimen Characteristics:** Inhomogeneous; solid; unknown crystallinity; dielectric; inorganic compound; powder;

**Chemical Name:** Basic cupric carbonate

**Source:** Kremer Pigmente GmbH

**Specimen Composition:** $CuCO_3 \cdot Cu(OH)_2$

**Form:** Ground pigment powder

**History and Significance:** A natural green to turquoise-green copper carbonate, which results from the erosion of copper deposits. It is one of the earliest known bright green pigments, and a dominant one until the mid-18th century. It was considered a fairly precious material. It consists of rather large spherical particles.

**As Received Condition:** Ground pigment powders were stored in a sealed glass vial in a wooden box, protected from daylight. Stored at room temperature.

**Analyzed Region:** Areas of $250 \times 250 \ \mu m^2$

**Ex Situ Preparation/Mounting:** Powder was deposited and pressed onto conductive double-sided tape attached to stainless steel $1 \times 1 \ cm^2$ plates. The resulting deposit of powder had a flat surface and was fixed in a suitable way for the vacuum chamber. The plate was directly mounted on a “backmount” sample holder (IONTOF).

**In Situ Preparation:** None

**Charge Control Conditions and Procedures:** A low energy electron flood gun was used. Bias voltage between 20 and -30 V. Flood gun filament current 2.35 A. Surface potential was corrected (sample dependent).

**Temp. During Analysis:** 300 K

**Pressure During Analysis:** Between $1 \times 10^{-5}$ and $1 \times 10^{-6}$ Pa

**Pre-analysis Beam Exposure:** $Ar_{1500-2000}$, 20 keV, $2 \times 10^{15}$ ions/cm$^2$

## SPECIMEN DESCRIPTION (ACCESSION # 01945)

**Specimen:** Verdigris, synthetic (Kremer Pigmente Ref. 44450)

**CAS Registry #:** 6046-93-1

**Specimen Characteristics:** Inhomogeneous; solid; unknown crystallinity; dielectric; inorganic compound; powder;

**Chemical Name:** Copper-(II)-acetate-1-hydrate

**Source:** Kremer Pigmente GmbH

**Specimen Composition:** $Cu(CH_3COO)_2 \cdot [Cu(OH)_2]_3 \cdot 2H_2O$

**Form:** Ground pigment powder

**History and Significance:** A family of synthetic pigments, containing variations of copper acetate, with green to blue-green hues. Synthesized since Antiquity, it is an acetate copper salt produced by the reaction of acetic acid with copper and has been particularly common in wine-growing regions. It has a characteristic vinegar odor. A better knowledge of the ion signal of Verdigris pigments is of interest. Indeed, considered unstable, it reacts with binders and other pigments forming soaps and other copper salts, respectively, making its identification in a painting often ambiguous. Degradation products result in a brown tint.

**As Received Condition:** Ground pigment powders were stored in a sealed glass vial in a wooden box, protected from daylight. Stored at room temperature.

**Analyzed Region:** Areas of $250 \times 250 \ \mu m^2$

**Ex Situ Preparation/Mounting:** Powder was deposited and pressed onto conductive double-sided tape attached to stainless steel $1 \times 1 \ cm^2$ plates. The resulting deposit of powder had a flat surface and was fixed in a suitable way for the vacuum chamber. The plate was directly mounted on a “backmount” sample holder (IONTOF).

**In Situ Preparation:** None

**Charge Control Conditions and Procedures:** A low energy electron flood gun was used. Bias voltage between 20 and -30 V. Flood gun filament current 2.35 A. Surface potential was corrected (sample dependent).

**Temp. During Analysis:** 300 K

**Pressure During Analysis:** Between $1 \times 10^{-5}$ and $1 \times 10^{-6}$ Pa

**Pre-analysis Beam Exposure:** $Ar_{1500-2000}$, 20 keV, $2 \times 10^{15}$ ions/cm$^2$

## SPECIMEN DESCRIPTION (ACCESSION # 01946)

**Specimen:** Zinc white (Kremer Pigmente Ref. 46300)

**CAS Registry #:** 1314-13-2

**Specimen Characteristics:** Inhomogeneous; solid; unknown crystallinity; dielectric; inorganic compound; powder;

**Chemical Name:** Zinc oxide

**Source:** Kremer Pigmente GmbH

**Specimen Composition:** ZnO

**Form:** Ground pigment powder

**History and Significance:** A widely used substitute for lead-containing whites that was first produced in the 19th century by Winsor & Newton (1834) with Michael Faraday.

**As Received Condition:** Ground pigment powders were stored in a sealed glass vial in a wooden box, protected from daylight. Stored at room temperature.

**Analyzed Region:** Areas of $250 \times 250 \ \mu m^2$

**Ex Situ Preparation/Mounting:** Powder was deposited and pressed onto conductive double-sided tape attached to stainless steel 1 cm × 1 cm plates. The resulting deposit of powder had a flat surface and was fixed in a suitable way for the vacuum
chamber. The plate was directly mounted on a “backmount”
sample holder (IONTOF).

**In Situ Preparation:** None

**Charge Control Conditions and Procedures:** A low energy electron flood gun was used. Bias voltage between 20 and -30 V. Flood gun filament current 2.35 A. Surface potential was corrected (sample dependent).

**Temp. During Analysis:** 300 K

**Pressure During Analysis:** Between $1 \times 10^{-5}$ and $1 \times 10^{-6}$ Pa

**Pre-analysis Beam Exposure:** $Ar_{1500-2000}$, 20 keV, $2 \times 10^{15}$ ions/cm$^2$

## INSTRUMENT CONFIGURATION

**Manufacturer and Model:** IONTOF, TOF SIMS IV

**Analyzer Type:** Time-of-flight

**Sample Rotation:** No

**Rotation Rate:** 0 rpm

**Oxygen Flood Source:** None

**Oxygen Flood Pressure:** N/A

**Other Flood Source:** None

**Other Flood Pressure:** N/A

**Unique Instrument Features Used:** None

**Energy Acceptance Window:** 20 eV

**Post-acceleration Voltage:** 10 000 eV

**Sample Bias:** 10–20 eV

**Specimen Normal-to-analyzer (Θe):** 0°

### Ion sources

#### Ion source 1 of 2

**Purpose of this Ion Source:** Analysis beam

**Ion Source Manufacturer:** IONTOF GmbH

**Ion Source Model:** Liquid metal ion gun (LMIG) with bismuth cluster (25 keV)

**Beam Mass Filter:** Yes

**Beam Species and Charge State:** $Bi_3^+$

**Beam Gating Used:** Double pulsed + Bunched

**Additional Beam Comments:** None

**Beam Voltage:** 25 000 eV

**Net Beam Voltage (impact voltage):** 25 000 eV

**Ion Pulse Width:** 0.8–1.2 ns

**Ion Pulse Rate:** 5–10 kHz

**DC Beam Current:** ~10 nA

**Pulsed Beam Current:** ~0.0004 nA

**Current Measurement Method:** Faraday cup

**Beam Diameter:** ~2 µm

**Beam Raster Size:** 250 × 250 µm$^2$

**Rotor Pixel Dimensions:** 128 × 128

**Beam Incident Angle:** 45°

**Source-to-Analyzer Angle:** 45°

#### Ion source 2 of 2

**Purpose of this Ion Source:** Sputtering beam

**Ion Source Manufacturer:** IONTOF GmbH

**Ion Source Model:** Argon GCIB

**Beam Mass Filter:** Yes

**Beam Species and Charge State:** $Ar_n^+$ with n = 1500–2000

**Beam Gating Used:** Wien filter

**Additional Beam Comments:** Used as sputter gun, not analysis mode.

**Beam Voltage:** 20 000 eV

**Net Beam Voltage (impact voltage):** 20 000 eV

**Ion Pulse Width:** N/A

**Ion Pulse Rate:** N/A

**DC Beam Current:** ~10 nA

**Pulsed Beam Current:** N/A

**Current Measurement Method:** Faraday cup

**Beam Diameter:** ~50 µm

**Beam Raster Size:** 500 × 500 µm$^2$

**Rotor Pixel Dimensions:** N/A

**Beam Incident Angle:** 45°

**Source-to-Analyzer Angle:** 45°

## ACKNOWLEDGMENTS

This work was financially supported by the Agence Nationale de la Recherche (Grant No. ANR-2015-CE29-0007 DEFIMAGE). C.B. has received funding from the European Union's Horizon Europe Research and Innovation Programme under the Marie Skłodowska-Curie Grant Agreement No. 101108506. The authors thank Sven Kayser and Matthias Kleine-Boymann (IONTOF GmbH) for providing extended access to the software SURFACE LAB 7.3 that allowed thorough processing of the data.

## AUTHOR DECLARATIONS

### Conflict of Interest

The authors have no conflicts to disclose.

### Author Contributions

**Caroline Bouvier:** Investigation (lead); Writing – original draft (lead). **Sebastiaan Van Nuffel:** Investigation (equal); Writing – review & editing (lead). **Alain Brunelle:** Conceptualization (lead); Supervision (equal); Writing – review & editing (equal).

## DATA AVAILABILITY

The data that support the findings of this study are available within the article and its supplementary material.

## REFERENCES

¹R. G. Cooks and K. L. Bush, *Int. J. Mass Spectrom.* **53**, 111 (1983).

²N. Eastaugh, V. Walsh, T. Chaplin, and R. Siddall, *Pigment Compendium: A Dictionary and Optical Microscopy of Historical Pigments*, 1st ed. (Routledge, London, 2008).

³E. Robert and L. Feller, *Artists' Pigments: A Handbook of Their History and Characteristics*, Vol. 1 (Archetype Publications, London, 1986).

⁴A. Roy, *Artists' Pigments: A Handbook of Their History and Characteristics*, Vol. 2 (Archetype Publications, London, 1993).

⁵E. W. FitzHugh, *Artists' Pigments: A Handbook of Their History and Characteristics*, Vol. 3 (Archetype Publications, London, 1997).

⁶J. R. Barnett, S. Miller, and E. Pearce, *Opt. Laser Technol.* **38**, 445 (2006).

⁷L. M. Smieska, R. Mullett, L. Ferri, and A. R. Woll, *Appl. Phys. A* **123**, 1 (2017).

⁸M. Price, *Leonardo* **33**, 281 (2000).
<table><caption>SPECTRAL FEATURES TABLE</caption><thead><tr><th>Spectrum ID #</th><th>Mass (Δm), Da</th><th>Species</th><th>Peak Assignment</th></tr></thead><tbody><tr><td rowspan="14">01939-01</td><td>38.963 (4.42)</td><td>K<sup>+</sup></td><td>–</td></tr><tr><td>51.022 (–12.4)</td><td>C<sub>4</sub>H<sub>3</sub><sup>+</sup></td><td>Charcoal</td></tr><tr><td>63.022 (–13.6)</td><td>C<sub>5</sub>H<sub>3</sub><sup>+</sup></td><td>Charcoal</td></tr><tr><td>77.042 (37.9)</td><td>C<sub>6</sub>H<sub>5</sub><sup>+</sup></td><td>Charcoal</td></tr><tr><td>91.053 (–14.9)</td><td>C<sub>7</sub>H<sub>7</sub><sup>+</sup></td><td>Charcoal</td></tr><tr><td>94.927 (–31.1)</td><td>K<sub>2</sub>OH<sup>+</sup></td><td>–</td></tr><tr><td>102.925 (–4.01)</td><td>KSO<sub>2</sub><sup>+</sup></td><td>–</td></tr><tr><td>112.896 (1.74)</td><td>K<sub>2</sub>Cl<sup>+</sup></td><td>–</td></tr><tr><td>115.052 (–15.7)</td><td>C<sub>9</sub>H<sub>7</sub><sup>+</sup></td><td>Charcoal</td></tr><tr><td>128.062 (2.43)</td><td>C<sub>10</sub>H<sub>8</sub><sup>+</sup></td><td>Charcoal</td></tr><tr><td>140.886 (–29.7)</td><td>K<sub>2</sub>PO<sub>2</sub><sup>+</sup></td><td>–</td></tr><tr><td>141.067 (–21.4)</td><td>C<sub>11</sub>H<sub>9</sub><sup>+</sup></td><td>Charcoal</td></tr><tr><td>196.840 (–35.0)</td><td>K<sub>3</sub>SO<sub>3</sub><sup>+</sup></td><td>–</td></tr><tr><td>212.834 (–40.0)</td><td>K<sub>3</sub>SO<sub>4</sub><sup>+</sup></td><td>–</td></tr></tbody></table>
<figure><img src="image_9.png" /></figure>

<table><tr><td>Accession #:</td><td>01939-01</td></tr><tr><td>■ Specimen:</td><td>Peach Black—Kremer Pigmente Ref. 12010</td></tr><tr><td>■ Technique:</td><td>SIMS</td></tr><tr><td>Instrument:</td><td>IONTOF, TOF SIMS IV</td></tr><tr><td>Analyzer Type:</td><td>Time-of-flight</td></tr><tr><td>Analyzer Mass Resolving Power:</td><td>1200 m/Δm</td></tr><tr><td>Mass Resolving Power Determined at:</td><td>27 Da</td></tr><tr><td>Species Used for Mass Calibration:</td><td>C<sup>+</sup>, K<sup>+</sup>, K<sub>2</sub>OH<sup>+</sup>, K<sub>2</sub>Cl<sup>+</sup></td></tr><tr><td>Specimen Normal-to-Analyzer:</td><td>0°</td></tr><tr><td>Source-to-Analyzer Angle:</td><td>45°</td></tr><tr><td>Primary Beam Ion Gun:</td><td>LMIG</td></tr><tr><td>Primary Ion Species:</td><td>Bi<sup>3+</sup></td></tr><tr><td>Primary Ion Dose:</td><td>4.35 × 10<sup>11</sup> ion/cm<sup>2</sup></td></tr><tr><td>Primary Ion Pulse Width:</td><td>0.8–1.2 ns</td></tr><tr><td>Primary Ion Pulse Rate:</td><td>5 kHz</td></tr><tr><td>Net Beam Voltage:</td><td>25 000 eV</td></tr><tr><td>Pulsed Beam Current:</td><td>0.000 13 nA</td></tr><tr><td>DC Beam Current:</td><td>10.4 nA</td></tr><tr><td>Beam Diameter:</td><td>~2 μm</td></tr><tr><td>Beam Raster Size:</td><td>250 × 250 μm<sup>2</sup></td></tr><tr><td>Beam Incident Angle:</td><td>45°</td></tr><tr><td>Secondary Source Polarity:</td><td>Positive</td></tr><tr><td>Mass Range Minimum:</td><td>0 Da</td></tr><tr><td>Mass Range Maximum:</td><td>3545 Da</td></tr><tr><td>Spectrum Dead Time Corrected:</td><td>Yes</td></tr><tr><td>Total Spectral Acquisition Time:</td><td>335 s</td></tr><tr><td>Comment:</td><td>The peak at m/z 102.925 attributed to KSO<sub>2</sub><sup>+</sup> can be distinguished from the peak at m/z 102.925 attributed to CaPO<sub>2</sub><sup>+</sup> found in Bone Black (#01940) using isotopic pattern matching.</td></tr></table>
<table><caption>SPECTRAL FEATURES TABLE</caption><thead><tr><th>Spectrum ID #</th><th>Mass (Δm), Da</th><th>Species</th><th>Peak Assignment</th></tr></thead><tbody><tr><td rowspan="20">01940-01</td><td>22.990 (23.4)</td><td>Na<sup>+</sup></td><td>–</td></tr><tr><td>23.984 (–20.6)</td><td>Mg<sup>+</sup></td><td>–</td></tr><tr><td>26.981 (–12.7)</td><td>Al<sup>+</sup></td><td>–</td></tr><tr><td>27.977 (7.35)</td><td>Si<sup>+</sup></td><td>–</td></tr><tr><td>38.963 (3.53)</td><td>K<sup>+</sup></td><td>–</td></tr><tr><td>39.962 (7.67)</td><td>Ca<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>55.934 (–6.43)</td><td>Fe<sup>+</sup></td><td>–</td></tr><tr><td>55.956 (–14.7)</td><td>CaO<sup>+</sup></td><td>–</td></tr><tr><td>56.964 (–12.6)</td><td>CaOH<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>95.919 (–8.30)</td><td>Ca(CaO)<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>102.925 (–7.34)</td><td>CaPO<sub>2</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>112.921 (–8.34)</td><td>(CaO)<sub>2</sub>H<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>118.922 (9.49)</td><td>PO<sub>2</sub>CaO<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>151.877 (–1.23)</td><td>Ca(CaO)<sub>2</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>158.884 (5.26)</td><td>PO<sub>2</sub>Ca<sub>2</sub>O<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>168.880 (–3.83)</td><td>(CaO)<sub>3</sub>H<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>174.880 (8.25)</td><td>PO<sub>2</sub>Ca<sub>2</sub>O<sub>2</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>207.836 (5.63)</td><td>Ca(CaO)<sub>3</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>214.843 (11.0)</td><td>PO<sub>2</sub>Ca<sub>3</sub>O<sub>2</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>224.837 (0.48)</td><td>(CaO)<sub>4</sub>H<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>230.838 (8.71)</td><td>PO<sub>2</sub>Ca<sub>3</sub>O<sub>3</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>263.793 (3.21)</td><td>Ca(CaO)<sub>4</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>270.802 (15.8)</td><td>PO<sub>2</sub>Ca<sub>4</sub>O<sub>3</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>280.796 (3.47)</td><td>(CaO)<sub>5</sub>H<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>286.794 (2.04)</td><td>PO<sub>2</sub>Ca<sub>4</sub>O<sub>4</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>319.751 (5.56)</td><td>Ca(CaO)<sub>5</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>326.761 (16.6)</td><td>PO<sub>2</sub>Ca<sub>5</sub>O<sub>4</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>336.754 (3.66)</td><td>(CaO)<sub>6</sub>H<sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>342.753 (6.05)</td><td>PO<sub>2</sub>Ca<sub>5</sub>O<sub>5</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>398.711 (7.16)</td><td>PO<sub>2</sub>Ca<sub>6</sub>O<sub>6</sub><sup>+</sup></td><td>Calcium phosphate</td></tr><tr><td>454.678 (26.3)</td><td>PO<sub>2</sub>Ca<sub>7</sub>O<sub>7</sub><sup>+</sup></td><td>Calcium phosphate</td></tr></tbody></table>
<figure><img src="image_10.png" /></figure>

<table><thead><tr><th>Accession #:</th><th>01940-01</th></tr></thead><tbody><tr><td>■ Specimen:</td><td>Bone Black—Kremer Pigmente Ref. 47100</td></tr><tr><td>■ Technique:</td><td>SIMS</td></tr><tr><td>Instrument:</td><td>IONTOF, TOF SIMS IV</td></tr><tr><td>Analyzer Type:</td><td>Time-of-flight</td></tr><tr><td>Analyzer Mass Resolving Power:</td><td>3500 m/Δm</td></tr><tr><td>Mass Resolving Power Determined at:</td><td>27 Da</td></tr><tr><td>Species Used for Mass Calibration:</td><td>Na<sup>+</sup>, Ca<sup>+</sup>, Ca<sub>2</sub>O<sup>+</sup>, Ca<sub>3</sub>O<sub>2</sub><sup>+</sup>, Ca<sub>4</sub>O<sub>3</sub><sup>+</sup>, Ca<sub>5</sub>O<sub>4</sub><sup>+</sup>, Ca<sub>6</sub>O<sub>5</sub><sup>+</sup></td></tr><tr><td>Specimen Normal-to-Analyzer:</td><td>0°</td></tr><tr><td>Source-to-Analyzer Angle:</td><td>45°</td></tr><tr><td>Primary Beam Ion Gun:</td><td>LMIG</td></tr><tr><td>Primary Ion Species:</td><td>Bi<sup>3+</sup></td></tr><tr><td>Primary Ion Dose:</td><td>4.37 × 10<sup>11</sup> ion/cm<sup>2</sup></td></tr><tr><td>Primary Ion Pulse Width:</td><td>0.8–1.2 ns</td></tr><tr><td>Primary Ion Pulse Rate:</td><td>5 kHz</td></tr><tr><td>Net Beam Voltage:</td><td>25 000 eV</td></tr><tr><td>Pulsed Beam Current:</td><td>0.000 15 nA</td></tr><tr><td>DC Beam Current:</td><td>14.7 nA</td></tr><tr><td>Beam Diameter:</td><td>~2 µm</td></tr><tr><td>Beam Raster Size:</td><td>250 × 250 µm<sup>2</sup></td></tr><tr><td>Beam Incident Angle:</td><td>45°</td></tr><tr><td>Secondary Source Polarity:</td><td>Positive</td></tr><tr><td>Mass Range Minimum:</td><td>0 Da</td></tr><tr><td>Mass Range Maximum:</td><td>3545 Da</td></tr><tr><td>Spectrum Dead Time Corrected:</td><td>Yes</td></tr><tr><td>Total Spectral Acquisition Time:</td><td>292 s</td></tr><tr><td>Comment:</td><td>The peak at m/z 102.925 attributed to CaPO<sub>2</sub><sup>+</sup> can be distinguished from the peak at m/z 102.925 attributed to KSO<sub>2</sub><sup>+</sup> found in Peach Black (#01939) using isotopic pattern matching.</td></tr></tbody></table>
<table><caption>SPECTRAL FEATURES TABLE</caption><thead><tr><th>Spectrum ID #</th><th>Mass (Δm), Da</th><th>Species</th><th>Peak Assignment</th></tr></thead><tbody><tr><td rowspan="20">01941-01</td><td>74.922 (13.4)</td><td>As<sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>90.914 (−22.6)</td><td>AsO<sup>+</sup></td><td>Arsenic oxide</td></tr><tr><td>106.891 (−27.9)</td><td>AsS<sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>138.863 (−15.7)</td><td>AsS<sub>2</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>181.814 (−6.79)</td><td>As<sub>2</sub>S<sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>207.972 (−17.8)</td><td>Pb<sup>+</sup></td><td>Natural impurity</td></tr><tr><td>213.783 (−16.5)</td><td>As<sub>2</sub>S<sub>2</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>245.756 (−10.3)</td><td>As<sub>2</sub>S<sub>3</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>256.734 (−8.30)</td><td>As<sub>3</sub>S<sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>272.748 (−3.46)</td><td>As<sub>3</sub>O<sup>+</sup></td><td>Arsenic oxide</td></tr><tr><td>288.726 (−0.90)</td><td>As<sub>3</sub>SO<sub>2</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub>/arsenic oxide</td></tr><tr><td>314.871 (4.83)</td><td>PbAsS<sup>+</sup></td><td>Natural impurity</td></tr><tr><td>320.678 (−7.97)</td><td>As<sub>3</sub>S<sub>3</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>346.832 (−27.5)</td><td>PbAsS<sub>2</sub><sup>+</sup></td><td>Natural impurity</td></tr><tr><td>352.653 (1.19)</td><td>As<sub>3</sub>S<sub>4</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>378.807 (−19.5)</td><td>PbAsS<sub>3</sub><sup>+</sup></td><td>Natural impurity</td></tr><tr><td>395.601 (−2.70)</td><td>As<sub>4</sub>S<sub>3</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>427.583 (19.8)</td><td>As<sub>4</sub>S<sub>4</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub></td></tr><tr><td>470.576 (−1.02)</td><td>As<sub>5</sub>O<sub>6</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub>/arsenic oxide</td></tr><tr><td>486.578 (12.6)</td><td>As<sub>5</sub>O<sub>7</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub>/arsenic oxide</td></tr><tr><td>502.575 (15.5)</td><td>As<sub>5</sub>O<sub>8</sub><sup>+</sup></td><td>α-As<sub>4</sub>S<sub>4</sub>/arsenic oxide</td></tr></tbody></table>
<figure><img src="image_11.png" /></figure>

<table><thead><tr><th>Accession #:</th><th>01941-01</th></tr></thead><tbody><tr><td>■ Specimen:</td><td>Realgar/red orpiment—Kremer Pigmente Ref. 10800</td></tr><tr><td>■ Technique:</td><td>SIMS</td></tr><tr><td>Instrument:</td><td>IONTOF, TOF SIMS IV</td></tr><tr><td>Analyzer Type:</td><td>Time-of-flight</td></tr><tr><td>Analyzer Mass Resolving Power:</td><td>3900 m/Δm</td></tr><tr><td>Mass Resolving Power Determined at:</td><td>27 Da</td></tr><tr><td>Species Used for Mass Calibration:</td><td>As<sup>+</sup>, AsS<sup>+</sup>, As<sub>2</sub>S<sub>2</sub><sup>+</sup>, AsPbS<sup>+</sup>, As<sub>3</sub>S<sub>3</sub><sup>+</sup></td></tr><tr><td>Specimen Normal-to-Analyzer:</td><td>0°</td></tr><tr><td>Source-to-Analyzer Angle:</td><td>45°</td></tr><tr><td>Primary Beam Ion Gun:</td><td>LMIG</td></tr><tr><td>Primary Ion Species:</td><td>Bi<sup>i</sup></td></tr><tr><td>Primary Ion Dose:</td><td>4.34 × 10<sup>11</sup> ion/cm<sup>2</sup></td></tr><tr><td>Primary Ion Pulse Width:</td><td>0.8–1.2 ns</td></tr><tr><td>Primary Ion Pulse Rate:</td><td>5 kHz</td></tr><tr><td>Net Beam Voltage:</td><td>25 000 eV</td></tr><tr><td>Pulsed Beam Current:</td><td>0.000 21 nA</td></tr><tr><td>DC Beam Current:</td><td>14.4 nA</td></tr><tr><td>Beam Diameter:</td><td>~2 µm</td></tr><tr><td>Beam Raster Size:</td><td>250 × 250 µm<sup>2</sup></td></tr><tr><td>Beam Incident Angle:</td><td>45°</td></tr><tr><td>Secondary Source Polarity:</td><td>Positive</td></tr><tr><td>Mass Range Minimum:</td><td>0 Da</td></tr><tr><td>Mass Range Maximum:</td><td>3545 Da</td></tr><tr><td>Spectrum Dead Time Corrected:</td><td>Yes</td></tr><tr><td>Total Spectral Acquisition Time:</td><td>207 s</td></tr><tr><td>Comment:</td><td>Unstable, sensitive to light and oxygen. All oxygen-containing ions were localized in the same round-shaped areas of about 10 µm diameter dispersed on the surface, allowing us to confidently determine if a species contained oxygen or only sulfur.</td></tr></tbody></table>
<table><caption>SPECTRAL FEATURES TABLE</caption><thead><tr><th>Spectrum ID #</th><th>Mass (Δm), Da</th><th>Species</th><th>Peak Assignment</th></tr></thead><tbody><tr><td rowspan="20">01942-01</td><td>22.990 (31.5)</td><td>Na<sup>+</sup></td><td>—</td></tr><tr><td>26.981 (−4.76)</td><td>Al<sup>+</sup></td><td>—</td></tr><tr><td>27.976 (−9.51)</td><td>Si<sup>+</sup></td><td>—</td></tr><tr><td>39.962 (5.09)</td><td>Ca<sup>+</sup></td><td>—</td></tr><tr><td>46.967 (−32.1)</td><td>PO<sup>+</sup></td><td>Zn<sub>3</sub>(PO<sub>4</sub>)<sub>2</sub></td></tr><tr><td>50.943 (−10.6)</td><td>V<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>55.956 (−20.7)</td><td>CaO<sup>+</sup></td><td>—</td></tr><tr><td>56.964 (−9.73)</td><td>CaOH<sup>+</sup></td><td>—</td></tr><tr><td>63.928 (−8.30)</td><td>Zn<sup>+</sup></td><td>—</td></tr><tr><td>66.939 (5.90)</td><td>VO<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>67.947 (8.58)</td><td>VOH<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>82.937 (47.8)</td><td>VO<sub>2</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>98.931 (29.6)</td><td>VO<sub>3</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>102.923 (−2.82)</td><td>CaPO<sub>2</sub><sup>+</sup></td><td>—</td></tr><tr><td>118.921 (−0.26)</td><td>CaOPO<sub>2</sub><sup>+</sup></td><td>—</td></tr><tr><td>122.896 (−2.51)</td><td>CaVO<sub>2</sub><sup>+</sup></td><td>—</td></tr><tr><td>126.893 (2.89)</td><td>ZnPO<sub>2</sub><sup>+</sup></td><td>Zn<sub>3</sub>(PO<sub>4</sub>)<sub>2</sub></td></tr><tr><td>133.876 (−8.97)</td><td>V<sub>2</sub>O<sub>2</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>138.893 (14.5)</td><td>CaVO<sub>3</sub><sup>+</sup></td><td>—</td></tr><tr><td>142.889 (9.85)</td><td>ZnPO<sub>3</sub><sup>+</sup></td><td>Zn<sub>3</sub>(PO<sub>4</sub>)<sub>2</sub></td></tr><tr><td>149.872 (−0.98)</td><td>V<sub>2</sub>O<sub>3</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>154.889 (21.3)</td><td>CaVO<sub>4</sub><sup>+</sup></td><td>—</td></tr><tr><td>158.881 (18.5)</td><td>V<sub>3</sub>H<sub>6</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>165.869 (10.5)</td><td>V<sub>2</sub>O<sub>4</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>174.875 (11.1)</td><td>V<sub>3</sub>H<sub>6</sub>O<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>181.865 (16.2)</td><td>V<sub>2</sub>O<sub>5</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>194.846 (−9.93)</td><td>Ca<sub>2</sub>VO<sub>4</sub><sup>+</sup></td><td>—</td></tr><tr><td>200.816 (−1.53)</td><td>V<sub>3</sub>O<sub>3</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>208.984 (18.6)</td><td>Bi<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>216.814 (13.1)</td><td>V<sub>3</sub>O<sub>4</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>224.977 (11.4)</td><td>BiO<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>232.810 (16.5)</td><td>V<sub>3</sub>O<sub>5</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>248.806 (19.8)</td><td>V<sub>3</sub>O<sub>6</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>275.913 (−21.0)</td><td>BiVO<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>291.913 (−2.34)</td><td>BiVO<sub>2</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>307.907 (−3.46)</td><td>BiVO<sub>3</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>417.967 (17.0)</td><td>Bi<sub>2</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>433.961 (14.6)</td><td>Bi<sub>2</sub>O<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>449.960 (21.2)</td><td>Bi<sub>2</sub>O<sub>2</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>516.893 (7.63)</td><td>Bi<sub>2</sub>VO<sub>3</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>532.895 (21.1)</td><td>Bi<sub>2</sub>VO<sub>4</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>548.869 (−18.6)</td><td>Bi<sub>2</sub>VO<sub>5</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>626.957 (26.1)</td><td>Bi<sub>3</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>642.941 (8.81)</td><td>Bi<sub>3</sub>O<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>658.935 (7.13)</td><td>Bi<sub>3</sub>O<sub>2</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>674.930 (6.75)</td><td>Bi<sub>3</sub>O<sub>3</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>741.873 (11.8)</td><td>Bi<sub>3</sub>VO<sub>4</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>835.936 (18.5)</td><td>Bi<sub>4</sub><sup>+</sup></td><td>BiVO<sub>4</sub></td></tr><tr><td>851.922 (7.25)</td><td>Bi<sub>4</sub>O<sup>+</sup></td><td>BiVO<sub>4</sub></td></tr></tbody></table>
<figure><img src="image_12.png" /></figure>

<table><thead><tr><th>Accession #:</th><th>01942-01</th></tr></thead><tbody><tr><td>■ Specimen:</td><td>Bristol Yellow—Kremer Pigmente Ref. 43111</td></tr><tr><td>■ Technique:</td><td>SIMS</td></tr><tr><td>■ Instrument:</td><td>IONTOF, TOF SIMS IV</td></tr><tr><td>Analyzer Type:</td><td>Time-of-flight</td></tr><tr><td>Analyzer Mass Resolving Power:</td><td>3500 m/Δm</td></tr><tr><td>Mass Resolving Power Determined at:</td><td>25 Da</td></tr><tr><td>Species Used for Mass Calibration:</td><td>Na<sup>+</sup>, Ca<sup>+</sup>, Ca<sub>2</sub>O<sup>+</sup>, Ca<sub>5</sub>O<sub>5</sub>H<sup>+</sup>, Ca<sub>6</sub>O<sub>6</sub>H<sup>+</sup></td></tr><tr><td>Specimen Normal-to-Analyzer:</td><td>0°</td></tr><tr><td>Source-to-Analyzer Angle:</td><td>45°</td></tr><tr><td>Primary Beam Ion Gun:</td><td>LMIG</td></tr><tr><td>Primary Ion Species:</td><td>Bi<sub>3</sub><sup>+</sup></td></tr><tr><td>Primary Ion Dose:</td><td>4.35 × 10<sup>11</sup> ion/cm<sup>2</sup></td></tr><tr><td>Primary Ion Pulse Width:</td><td>0.8–1.2 ns</td></tr><tr><td>Primary Ion Pulse Rate:</td><td>5 kHz</td></tr><tr><td>Net Beam Voltage:</td><td>25 000 eV</td></tr><tr><td>Pulsed Beam Current:</td><td>0.000 17 nA</td></tr><tr><td>DC Beam Current:</td><td>15.1 nA</td></tr><tr><td>Beam Diameter:</td><td>~2 µm</td></tr><tr><td>Beam Raster Size:</td><td>250 × 250 µm<sup>2</sup></td></tr><tr><td>Beam Incident Angle:</td><td>45°</td></tr><tr><td>Secondary Source Polarity:</td><td>Positive</td></tr><tr><td>Mass Range Minimum:</td><td>0 Da</td></tr><tr><td>Mass Range Maximum:</td><td>3545 Da</td></tr><tr><td>Spectrum Dead Time Corrected:</td><td>Yes</td></tr><tr><td>Total Spectral Acquisition Time:</td><td>256 s</td></tr></tbody></table>
<table><caption>SPECTRAL FEATURES TABLE</caption><thead><tr><th>Spectrum ID #</th><th>Mass (Δm), Da</th><th>Species</th><th>Peak Assignment</th></tr></thead><tbody><tr><td rowspan="20">01943-01</td><td>26.980 (−31.2)</td><td>Al+</td><td>–</td></tr><tr><td>38.965 (42.0)</td><td>K+</td><td>–</td></tr><tr><td>62.928 (−10.3)</td><td>Cu+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>106.915 (−34.4)</td><td>CO<sub>2</sub>Cu+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>118.913 (−49.5)</td><td>Cu<sub>2</sub>O<sub>2</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>125.857 (−10.8)</td><td>Cu<sub>2</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>137.901 (−23.8)</td><td>Ba+</td><td>Ba-rich impurity found in natural azurite<sup>7</sup></td></tr><tr><td>141.852 (−11.4)</td><td>Cu<sub>2</sub>O+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>154.906 (−7.22)</td><td>BaOH+</td><td>Ba-rich impurity found in natural azurite</td></tr><tr><td>188.790 (6.94)</td><td>Cu<sub>3</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>204.781 (−10.8)</td><td>Cu<sub>3</sub>O+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>214.810 (27.4)</td><td>Cu<sub>3</sub>C<sub>2</sub>H<sub>2</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>264.762 (−22.7)</td><td>Cu<sub>3</sub>O<sub>2</sub>CO<sub>2</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>276.777 (34.4)</td><td>Cu<sub>3</sub>C<sub>2</sub>O<sub>4</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>283.701 (−24.9)</td><td>Cu<sub>4</sub>O<sub>2</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>291.802 (−8.48)</td><td>Ba<sub>2</sub>O+</td><td>Ba-rich impurity found in natural azurite</td></tr><tr><td>308.800 (−23.7)</td><td>Ba<sub>2</sub>O<sub>2</sub>H+</td><td>Ba-rich impurity found in natural azurite</td></tr><tr><td>330.648 (15.7)</td><td>Cu<sub>5</sub>O+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>346.631 (−18.8)</td><td>Cu<sub>5</sub>O<sub>2</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>362.625 (−20.1)</td><td>Cu<sub>5</sub>O<sub>3</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr><tr><td>425.551 (−26.1)</td><td>Cu<sub>6</sub>O<sub>3</sub>+</td><td>Cu<sub>3</sub>(CO<sub>3</sub>)<sub>2</sub>(OH)<sub>2</sub></td></tr></tbody></table>
<figure><img src="image_13.png" /></figure>

<table><thead><tr><th>Accession #:</th><th>01943-01</th></tr></thead><tbody><tr><td>■ Specimen:</td><td>Azurite—Kremer Pigmente Ref. 10207</td></tr><tr><td>■ Technique:</td><td>SIMS</td></tr><tr><td>Instrument:</td><td>IONTOF, TOF SIMS IV</td></tr><tr><td>Analyzer Type:</td><td>Time-of-flight</td></tr><tr><td>Analyzer Mass Resolving Power:</td><td>2000 m/Δm</td></tr><tr><td>Mass Resolving Power Determined at:</td><td>27 Da</td></tr><tr><td>Species Used for Mass Calibration:</td><td>Na<sup>+</sup>, Cu<sup>+</sup>, Cu<sub>2</sub>OH<sup>+</sup>, Cu<sub>3</sub>O<sup>+</sup>, <sup>65</sup>CuCu<sub>3</sub>O<sub>2</sub><sup>+</sup>, <sup>65</sup>CuCu<sub>4</sub>O<sub>2</sub><sup>+</sup></td></tr><tr><td>Specimen Normal-to-Analyzer:</td><td>0°</td></tr><tr><td>Source-to-Analyzer Angle:</td><td>45°</td></tr><tr><td>Primary Beam Ion Gun:</td><td>LMIG</td></tr><tr><td>Primary Ion Species:</td><td>Bi<sub>3</sub><sup>+</sup></td></tr><tr><td>Primary Ion Dose:</td><td>4.35 × 10<sup>11</sup> ion/cm<sup>2</sup></td></tr><tr><td>Primary Ion Pulse Width:</td><td>0.8–1.2 ns</td></tr><tr><td>Primary Ion Pulse Rate:</td><td>5 kHz</td></tr><tr><td>Net Beam Voltage:</td><td>25 000 eV</td></tr><tr><td>Pulsed Beam Current:</td><td>0.000 13 nA</td></tr><tr><td>DC Beam Current:</td><td>10.4 nA</td></tr><tr><td>Beam Diameter:</td><td>~2 µm</td></tr><tr><td>Beam Raster Size:</td><td>250 × 250 µm<sup>2</sup></td></tr><tr><td>Beam Incident Angle:</td><td>45°</td></tr><tr><td>Secondary Source Polarity:</td><td>Positive</td></tr><tr><td>Mass Range Minimum:</td><td>0 Da</td></tr><tr><td>Mass Range Maximum:</td><td>3545 Da</td></tr><tr><td>Spectrum Dead Time Corrected:</td><td>Yes</td></tr><tr><td>Total Spectral Acquisition Time:</td><td>335 s</td></tr><tr><td>Comment:</td><td>Organic contamination, likely from pigment processing.<sup>8</sup> Additional series of peaks are detected, with lower intensity. Some can be attributed to Cu<sub>n</sub>O<sub>4</sub><sup>+</sup> with n = 7–8. Other can be attributed to Ba<sub>n</sub>O<sub>n</sub>H<sup>+</sup> with n = 3–4 from Ba-rich impurities.</td></tr></tbody></table>
<table><caption>SPECTRAL FEATURES TABLE</caption><thead><tr><th>Spectrum ID #</th><th>Mass (Δm), Da</th><th>Species</th><th>Peak Assignment</th></tr></thead><tbody><tr><td rowspan="24">01944-01</td><td>22.990 (29.8)</td><td>Na<sup>+</sup></td><td>—</td></tr><tr><td>26.981 (−4.25)</td><td>Al<sup>+</sup></td><td>—</td></tr><tr><td>38.964 (26.9)</td><td>K<sup>+</sup></td><td>—</td></tr><tr><td>62.928 (−18.0)</td><td>Cu<sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>79.958 (26.4)</td><td>CuNH<sub>3</sub><sup>+</sup></td><td>—</td></tr><tr><td>90.929 (−11.2)</td><td>CuC<sub>2</sub>H<sub>4</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>106.916 (−25.9)</td><td>CO<sub>2</sub>Cu<sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>125.857 (−15.3)</td><td>Cu<sub>2</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>141.852 (−9.92)</td><td>Cu<sub>2</sub>O<sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>160.829 (8.01)</td><td>Cu<sub>2</sub>Cl<sup>+</sup></td><td>—</td></tr><tr><td>188.787 (−8.78)</td><td>Cu<sub>3</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>204.781 (−11.5)</td><td>Cu<sub>3</sub>O<sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>220.775 (−16.1)</td><td>Cu<sub>3</sub>O<sub>2</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>264.757 (−42.9)</td><td>Cu<sub>3</sub>O<sub>2</sub>CO<sub>2</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>283.704 (−13.0)</td><td>Cu<sub>4</sub>O<sub>2</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>302.685 (11.3)</td><td>Cu<sub>4</sub>OCl<sup>+</sup></td><td>—</td></tr><tr><td>314.647 (−1.96)</td><td>Cu<sub>5</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>330.638 (−12.6)</td><td>Cu<sub>5</sub>O<sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>346.628 (−27.3)</td><td>Cu<sub>5</sub>O<sub>2</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>362.624 (−21.8)</td><td>Cu<sub>5</sub>O<sub>3</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr><tr><td>425.555 (−16.9)</td><td>Cu<sub>6</sub>O<sub>3</sub><sup>+</sup></td><td>CuCO<sub>3</sub>·Cu(OH)<sub>2</sub></td></tr></tbody></table>
<figure><img src="image_14.png" /></figure>

<table><tr><td>Accession #:</td><td>01944-01</td></tr><tr><td>■ Specimen:</td><td>Malachite, natural—Kremer Pigmente Ref. 10300</td></tr><tr><td>■ Technique:</td><td>SIMS</td></tr><tr><td>Instrument:</td><td>IONTOF, TOF SIMS IV</td></tr><tr><td>Analyzer Type:</td><td>Time-of-flight</td></tr><tr><td>Analyzer Mass Resolving Power:</td><td>2100 m/Δm</td></tr><tr><td>Mass Resolving Power Determined at:</td><td>27 Da</td></tr><tr><td>Species Used for Mass Calibration:</td><td>Na<sup>+</sup>, Cu<sup>+</sup>, Cu<sub>2</sub>OH<sup>+</sup>, Cu<sub>3</sub>O<sup>+</sup>, <sup>65</sup>CuCu<sub>3</sub>O<sub>2</sub>, <sup>65</sup>CuCu<sub>4</sub>O<sub>2</sub></td></tr><tr><td>Specimen Normal-to-Analyzer:</td><td>0°</td></tr><tr><td>Source-to-Analyzer Angle:</td><td>45°</td></tr><tr><td>Primary Beam Ion Gun:</td><td>LMIG</td></tr><tr><td>Primary Ion Species:</td><td>Bi<sub>3</sub><sup>+</sup></td></tr><tr><td>Primary Ion Dose:</td><td>4.35 × 10<sup>11</sup> ion/cm<sup>2</sup></td></tr><tr><td>Primary Ion Pulse Width:</td><td>0.8–1.2 ns</td></tr><tr><td>Primary Ion Pulse Rate:</td><td>5 kHz</td></tr><tr><td>Net Beam Voltage:</td><td>25 000 eV</td></tr><tr><td>Pulsed Beam Current:</td><td>0.000 13 nA</td></tr><tr><td>DC Beam Current:</td><td>10.4 nA</td></tr><tr><td>Beam Diameter:</td><td>~2 μm</td></tr><tr><td>Beam Raster Size:</td><td>250 × 250 μm</td></tr><tr><td>Beam Incident Angle:</td><td>45°</td></tr><tr><td>Secondary Source Polarity:</td><td>Positive</td></tr><tr><td>Mass Range Minimum:</td><td>0 Da</td></tr><tr><td>Mass Range Maximum:</td><td>3545 Da</td></tr><tr><td>Spectrum Dead Time Corrected:</td><td>Yes</td></tr><tr><td>Total Spectral Acquisition Time:</td><td>335 s</td></tr><tr><td>Comment:</td><td>Additional series of peaks are commonly detected in this compound, with lower intensity. They can be attributed to other Cu<sub>x</sub>O<sub>y</sub>.</td></tr></table>
<table><caption>SPECTRAL FEATURES TABLE</caption><thead><tr><th>Spectrum ID #</th><th>Mass (Δm), Da</th><th>Species</th><th>Peak Assignment</th></tr></thead><tbody><tr><td rowspan="20">01945-01</td><td>15.023 (−24.0)</td><td>CH<sub>3</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>43.017 (−18.3)</td><td>C<sub>2</sub>H<sub>3</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>62.931 (29.0)</td><td>Cu<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>77.956 (47.4)</td><td>CH<sub>3</sub>Cu<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>80.941 (17.0)</td><td>CuOH<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>88.943 (−15.0)</td><td>CuC<sub>2</sub>H<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>90.924 (−0.84)</td><td>CuCO<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>104.938 (−14.8)</td><td>CuC<sub>2</sub>H<sub>2</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>106.920 (11.2)</td><td>CuCO<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>122.949 (−10.4)</td><td>CuC<sub>2</sub>H<sub>4</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>125.857 (−10.2)</td><td>Cu<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>140.882 (−3.47)</td><td>CH<sub>3</sub>Cu<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>142.865 (22.0)</td><td>Cu<sub>2</sub>OH<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>150.866 (−6.44)</td><td>Cu<sub>2</sub>C<sub>2</sub>H<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>166.863 (6.76)</td><td>Cu<sub>2</sub>C<sub>2</sub>OH<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>184.873 (5.96)</td><td>Cu<sub>2</sub>C<sub>2</sub>H<sub>3</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>188.788 (0.93)</td><td>Cu<sub>3</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>204.786 (15.5)</td><td>Cu<sub>3</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>212.787 (−4.56)</td><td>Cu<sub>3</sub>O<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>222.796 (−8.43)</td><td>Cu<sub>3</sub>O<sub>2</sub>H<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>228.786 (13.8)</td><td>Cu<sub>3</sub>C<sub>2</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>243.897 (47.9)</td><td>Cu<sub>2</sub>C<sub>4</sub>H<sub>6</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>264.759 (−35.2)</td><td>Cu<sub>3</sub>O<sub>2</sub>CO<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>264.813 (32.1)</td><td>Cu<sub>3</sub>OC<sub>2</sub>H<sub>4</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>283.710 (8.67)</td><td>Cu<sub>4</sub>O<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>284.718 (8.98)</td><td>Cu<sub>4</sub>O<sub>2</sub>H<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>292.718 (−8.63)</td><td>Cu<sub>4</sub>C<sub>2</sub>OH<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>306.810 (−17.3)</td><td>Cu<sub>3</sub>C<sub>4</sub>H<sub>6</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>323.811 (−20.7)</td><td>Cu<sub>3</sub>C<sub>4</sub>H<sub>7</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>326.718 (−25.8)</td><td>Cu<sub>4</sub>OC<sub>2</sub>H<sub>3</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>330.641 (−3.33)</td><td>Cu<sub>5</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>346.631 (−17.0)</td><td>Cu<sub>5</sub>O<sub>2</sub><sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub>·[Cu(OH)<sub>2</sub>]<sub>3</sub>·2H<sub>2</sub>O</td></tr><tr><td>365.821 (−20.0)</td><td>Cu<sub>3</sub>C<sub>6</sub>H<sub>9</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>381.817 (−16.7)</td><td>Cu<sub>3</sub>OC<sub>6</sub>H<sub>9</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>406.646 (−30.6)</td><td>Cu<sub>5</sub>C<sub>2</sub>H<sub>4</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>424.834 (−17.5)</td><td>Cu<sub>3</sub>C<sub>8</sub>H<sub>12</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>428.753 (−10.7)</td><td>Cu<sub>4</sub>C<sub>6</sub>H<sub>9</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>448.663 (−12.5)</td><td>Cu<sub>5</sub>OC<sub>4</sub>H<sub>6</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>483.840 (−31.6)</td><td>Cu<sub>3</sub>C<sub>10</sub>H<sub>15</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>503.752 (−28.6)</td><td>Cu<sub>4</sub>OC<sub>8</sub>H<sub>12</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>570.615 (5.87)</td><td>Cu<sub>6</sub>OC<sub>6</sub>H<sub>9</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr><tr><td>696.504 (47.0)</td><td>Cu<sub>8</sub>OC<sub>6</sub>H<sub>9</sub>O<sup>+</sup></td><td>Cu(CH<sub>3</sub>COO)<sub>2</sub></td></tr></tbody></table>
<figure><img src="image_15.png" /></figure>

<table><tr><td>Accession #:</td><td>01945-01</td></tr><tr><td>Specimen:</td><td>Verdigris, synthetic—Kremer Pigmente Ref. 44450</td></tr><tr><td>Technique:</td><td>SIMS</td></tr><tr><td>Instrument:</td><td>IONTOF, TOF SIMS IV</td></tr><tr><td>Analyzer Type:</td><td>Time-of-flight</td></tr><tr><td>Analyzer Mass Resolving Power:</td><td>3800 m/Δm</td></tr><tr><td>Mass Resolving Power Determined at:</td><td>27 Da</td></tr><tr><td>Species Used for Mass Calibration:</td><td>Na<sup>+</sup>, Cu<sup>+</sup>, Cu<sub>2</sub>OH<sup>+</sup>, Cu<sub>3</sub>O<sup>+</sup>, <sup>65</sup>CuCu<sub>3</sub>O<sub>2</sub><sup>+</sup>, <sup>65</sup>CuCu<sub>4</sub>O<sub>2</sub><sup>+</sup></td></tr><tr><td>Specimen Normal-to-Analyzer:</td><td>0°</td></tr><tr><td>Source-to-Analyzer Angle:</td><td>45°</td></tr><tr><td>Primary Beam Ion Gun:</td><td>LMIG</td></tr><tr><td>Primary Ion Species:</td><td>Bi<sup>+</sup></td></tr><tr><td>Primary Ion Dose:</td><td>1.0 × 10<sup>13</sup> ion/cm<sup>2</sup></td></tr><tr><td>Primary Ion Pulse Width:</td><td>0.8–1.2 ns</td></tr><tr><td>Primary Ion Pulse Rate:</td><td>6.7 kHz</td></tr><tr><td>Net Beam Voltage:</td><td>25 000 eV</td></tr><tr><td>Pulsed Beam Current:</td><td>0.000 31 nA</td></tr><tr><td>DC Beam Current:</td><td>13.2 nA</td></tr><tr><td>Beam Diameter:</td><td>~2 µm</td></tr><tr><td>Beam Raster Size:</td><td>100 × 100 µm<sup>2</sup></td></tr><tr><td>Beam Incident Angle:</td><td>45°</td></tr><tr><td>Secondary Source Polarity:</td><td>Positive</td></tr><tr><td>Mass Range Minimum:</td><td>0 Da</td></tr><tr><td>Mass Range Maximum:</td><td>1996 Da</td></tr><tr><td>Spectrum Dead Time Corrected:</td><td>Yes</td></tr><tr><td>Total Spectral Acquisition Time:</td><td>617 s</td></tr><tr><td>Comment:</td><td>Grains were not flat, and topography impacted the mass resolution.</td></tr></table>
<table><caption>SPECTRAL FEATURES TABLE</caption><thead><tr><th>Spectrum ID #</th><th>Mass (Δm), Da</th><th>Species</th><th>Peak Assignment</th></tr></thead><tbody><tr><td rowspan="20">01946-01</td><td>63.928 (−4.74)</td><td>Zn<sup>+</sup></td><td>ZnO</td></tr><tr><td>79.926 (24.9)</td><td>ZnO<sup>+</sup></td><td>ZnO</td></tr><tr><td>80.934 (33.0)</td><td>ZnOH<sup>+</sup></td><td>ZnO</td></tr><tr><td>127.858 (3.66)</td><td>Zn<sub>2</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>143.854 (9.57)</td><td>Zn(ZnO)<sup>+</sup></td><td>ZnO</td></tr><tr><td>144.861 (4.73)</td><td>Zn(ZnOH)<sup>+</sup></td><td>ZnO</td></tr><tr><td>159.849 (9.94)</td><td>(ZnO)<sub>2</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>160.857 (12.0)</td><td>(ZnO)<sub>2</sub>H<sup>+</sup></td><td>ZnO</td></tr><tr><td>191.789 (8.58)</td><td>Zn<sub>3</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>207.783 (6.72)</td><td>Zn<sub>3</sub>O<sup>+</sup></td><td>ZnO</td></tr><tr><td>223.777 (1.53)</td><td>Zn(ZnO)<sub>2</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>239.772 (−0.48)</td><td>(ZnO)<sub>3</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>240.779 (−2.54)</td><td>(ZnO)<sub>3</sub>H<sup>+</sup></td><td>ZnO</td></tr><tr><td>287.708 (7.95)</td><td>Zn<sub>4</sub>O<sub>2</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>303.697 (−11.3)</td><td>Zn(ZnO)<sub>3</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>319.690 (−16.7)</td><td>(ZnO)<sub>4</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>320.701 (−9.34)</td><td>(ZnO)<sub>4</sub>H<sup>+</sup></td><td>ZnO</td></tr><tr><td>383.627 (6.36)</td><td>Zn(ZnO)<sub>4</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>399.622 (6.27)</td><td>(ZnO)<sub>5</sub><sup>+</sup></td><td>ZnO</td></tr><tr><td>400.634 (16.0)</td><td>(ZnO)<sub>5</sub>H<sup>+</sup></td><td>ZnO</td></tr></tbody></table>
<figure><img src="image_16.png" /></figure>

<table><thead><tr><th>Accession #:</th><th>01946-01</th></tr></thead><tbody><tr><td>■ Specimen:</td><td>Zinc White—Kremer Pigmente Ref. 46300</td></tr><tr><td>■ Technique:</td><td>SIMS</td></tr><tr><td>Instrument:</td><td>IONTOF, TOF SIMS IV</td></tr><tr><td>Analyzer Type:</td><td>Time-of-flight</td></tr><tr><td>Analyzer Mass Resolving Power:</td><td>4200 m/Δm</td></tr><tr><td>Mass Resolving Power Determined at:</td><td>27 Da</td></tr><tr><td>Species Used for Mass Calibration:</td><td>Na<sup>+</sup> Zn<sup>+</sup> Zn<sub>2</sub>O<sub>2</sub><sup>+</sup> Zn<sub>3</sub>O<sub>3</sub><sup>+</sup> <sup>66</sup>Zn<sup>68</sup>ZnZn<sub>2</sub>O<sub>4</sub><sup>+</sup>, <sup>66</sup>Zn<sup>68</sup>ZnZn<sub>3</sub>O<sub>5</sub><sup>+</sup></td></tr><tr><td>Specimen Normal-to-Analyzer:</td><td>0°</td></tr><tr><td>Source-to-Analyzer Angle:</td><td>45°</td></tr><tr><td>Primary Beam Ion Gun:</td><td>LMIG</td></tr><tr><td>Primary Ion Species:</td><td>Bi<sub>3</sub><sup>+</sup></td></tr><tr><td>Primary Ion Dose:</td><td>4.37 × 10<sup>11</sup> ion/cm<sup>2</sup></td></tr><tr><td>Primary Ion Pulse Width:</td><td>0.8–1.2 ns</td></tr><tr><td>Primary Ion Pulse Rate:</td><td>5 kHz</td></tr><tr><td>Net Beam Voltage:</td><td>25 000 eV</td></tr><tr><td>Pulsed Beam Current:</td><td>0.000 15 nA</td></tr><tr><td>DC Beam Current:</td><td>14.7 nA</td></tr><tr><td>Beam Diameter:</td><td>~2 µm</td></tr><tr><td>Beam Raster Size:</td><td>250 × 250 µm<sup>2</sup></td></tr><tr><td>Beam Incident Angle:</td><td>45°</td></tr><tr><td>Secondary Source Polarity:</td><td>Positive</td></tr><tr><td>Mass Range Minimum:</td><td>0 Da</td></tr><tr><td>Mass Range Maximum:</td><td>3545 Da</td></tr><tr><td>Spectrum Dead Time Corrected:</td><td>Yes</td></tr><tr><td>Total Spectral Acquisition Time:</td><td>293 s</td></tr><tr><td>Comment:</td><td>Distinctive isotopic pattern for Zn. Exogenous organic contamination. Peaks attributed to (ZnO)<sub>x</sub> are commonly present up to x = 9, with lower intensity.</td></tr></tbody></table>